Effect of Intra-Orifice Barriers on the Fracture Resistance of Endodontically Treated Teeth – An Ex-Vivo Study
Shaheen Aboobaker1, Baiju Gopalan Nair2, Rajesh Gopal3, Sandeep Jituri4, Fazalu Rahman Pothu Veetil5
ABSTRACT Introduction: The purpose of this study was to evaluate and compare the fracture resistance of roots obturated with guttapercha using bonded amalgam, GC Light cure GIC (resin modified glass ionomer cement) and Tetric N Flow (flowable hybrid composite) as different intra orifice barriers. Materials and Methods: Eighty freshly extracted mandibular premolars with straight roots were reduced to 14 mm from the coronal aspect. All canals were enlarged to size 30 and specimens were obturated with gutta percha cones, except for control group specimens the coronal 3 mm of root fillings of all other group specimens were removed with the aid of heated plugger. All samples were randomly divided into 4 groups of 20 specimens each. They were control, Fuji GC LC GIC, Tetric N Flow and Bonded Amalgam. After the placement of the intra orifice barrier
materials, specimens stored at 37oC and 100% humidity for one week to allow the materials to set completely. After one week, all the groups were subjected to fracture resistance testing by using Universal testing machine. Results: Data was analysed for significance by ANOVA (Analysis of variance) and further pair wise comparison was performed by Benferroni test. Level of significance was taken as 0.05. Tetric N Flow group showed better fracture resistance as compared to all other groups and Control group is least among the groups. Fracture resistance of Tetric N Flow compared with bonded amalgam was statistically significant. Conclusion: Tetric N Flow and Fuji GC LC GIC can be used as intra-orifice barriers with good fracture resistance in endodon tically treated teeth.
Keywords: Bonded amalgam, Flowable composite, Glass ionomer cement, Intra-orifice barriers, LC GIC (light cure glass ionomer cement)
AIMS AND OBJECTIVES
Root canal therapy has provided dentistry with the ability to retain the teeth that just a few decades ago would have been extracted without hesitation. However, endodontically treated teeth are considered to be more susceptible to fracture than vital teeth. After the completion of endodontic treatment, restoration and protection of the remaining tooth structure is compulsory.
The aim and objective of this study is to compare and evaluate the fracture resistance of roots obturated with guttapercha using bonded amalgam, GC Light cure GIC (resin modified glass ionomer cement) and Tetric N Flow (flowable hybrid composite) as different Intra orifice barriers.
Non-restored, endodontically treated teeth are more prone to coronal leakage and fracture, which can lead to bacterial contamination and even failure of root canal therapy. Numerous clinical studies have shown that 11%- 13% of extracted teeth with endodontic treatment are associated with vertical root fractures . The reason often cited is removal of tooth structure during endodontic treatment and dehydration of dentin. The major goal of endodontic therapy should be reinforcement of the residual tooth structure . Since the retention of an adhesive restoration is based on micromechanical retention and does not require macro-retentive elements, minimal invasive preparation with maximal conservation of dentinal tissue can be realized. Coronal reinforcement of the tooth has been demonstrated through bonded restorations.
MATERIALs AND METHODS
Thus there is a need for different materials and/or techniques to overcome the shortcomings of current endodontic filling materials such as guttapercha or resilon to reinforce roots that is known as intra-orifice barriers. Intra-orifice barrier is an efficient alternative method to decrease coronal leakage in endodontically treated teeth . This procedure includes placing additional material into the canal orifices immediately after removal of the coronal portion of gutta-percha and sealer . Swartz et al., stated that “failure rate of endodontically treated teeth was almost double in cases without adequate post endodontic restoration” .
Soft tissue & calculus were mechanically removed from the root surface of 80 selected specimens [Table/Fig-1]. The teeth were reduced to 14 mm from the coronal aspect to standardize the specimens. After that all specimens were examined under a stereomicroscope to ensure the absence of cracks. A size 10 K-type file was placed into the canal until it was visible at the apical foramen. The working length was established 1 mm short of this length.
Journal of Clinical and Diagnostic Research. 2015 Feb, Vol-9(2): ZC17-ZC20
1. Selection of Specimens Human single canal mandibular premolars extracted for orthodontic purposes were collected from the department of Oral & Maxillofacial Surgery, Yenepoya Dental College, Mangalore, Karnataka, India. Inclusion Criteria: Eighty freshly extracted mandibular premolars selected on the basis of their macroscopically similar size and straight roots reduce to 14 mm from the coronal aspect. Exclusion Criteria: Teeth with fracture, craze lines and curved roots excluded.
2. Specimen Preparation
3. Canal Preparation The root canals instrumentation done with 0.06 taper Hero shaper rotory files in conjunction with RC-Prep lubrication and 2ml of 17
Shaheen Aboobaker et al., Effect of Intra-orifice Barriers On The Fracture Resistance of Endodontically Treated Teeth – An Ex-Vivo Study
[Table/Fig-1]: 80 selected mandibular premolars were arranged [Table/Fig-2]: Root canals were cleaned and shaped with rotory instruments [Table/Fig-3]: Tooth mounted in a self cure acrylic block
5.25% sodium hypochlorite irrigation between each files. All canals enlarged to ISO size 30 to the working length [Table/Fig-2]. The root canals had a final irrigation of 5 ml 17 % EDTA and 5 ml 2.5% NaOCl, after which the canals flushed with distilled water to avoid the prolonged effect of EDTA (RC- Prep) and NaOCl. The canals subsequently dried with paper points.
4. Canal Obturation
6. Fracture Strength Test The apical root ends were embedded along their long axis in selfcuring acrylic blocks, prepared from Leukhardts L-pieces mould leaving 9 mm of each root exposed [Table/Fig-3]. Thereafter, the specimens were mounted in a universal testing machine [Table/Fig-4] (Manipal college of dental sciences, manipal). A custom stainless steel loading fixture with a 2-mm spherical tip was centered over the canal opening [Table/Fig-5]. A compressive force was applied at a crosshead speed of 1 mm/min until fracture occurred. The
The root canal of each tooth was dried with paper points. AH plus sealer was mixed according to the manufacturer’s instructions. Root canal was coated with sealer and obturated with guttapercha cones of 0.06 taper single cones.
5. Placement of Intra Orifice Barriers Except for control group specimens the coronal 3 mm of root fillings of all other group specimens removed with the aid of heated finger plugger and verified with the help of william’s periodontal probe. Obturated specimens divided with respect to the intra orifice barrier material placed over the root canal fillings into the following groups.
GROUP 1: NO BARRIER (CONTROL) In this group, there were no removal of gutta-percha and no placement of intra-orifice barriers.
GROUP 2: FUJI GC LC GIC The specified amounts of powder and liquid dispensed onto the paper pad in the ratio of 3:1, then divided the powder into two equal parts. Mixed the first portion into the liquid with agate spatula and added the second portion into the remaining liquid. Mixed GIC (FUJI GC RESIN MODIFIED GIC) placed into the canal orifices and it was cured for 20 seconds with Blue phase C5 curing light (Ivoclar Vivadent).
GROUP 3: TETRIC N FLOW Prior to the restoration with composite, the root canal orifices were etched with 37% phosphoric acid (scotch bond etchant) for 15-20 sec. Then the surface was rinsed with water and the excess water was removed with an air syringe. Then the Adper Single bond 2(3M) adhesive was applied to enamel and dentine and was light cured for 10 sec. Finally placed the flowable hyrid composite (Ivoclar vivadent) and cured for 20 sec.
GROUP 4: BONDED AMALGAM Prior to the restoration with amalgam, mixed the equal amounts of ED PRIMER II A and B (Kuraray), applied with super fine microbrushes on the canal orifices and waited for 30 sec and air dried it. Then dispensed the equal amounts of Panavia F2.0 (Kuraray) luting paste A & B mixed and placed into root canal orifices. Then the amalgam was triturated in an amalgamator and the condensation was commenced immediately. Removed the excess cement and cured for 20 sec. The specimens of all groups were stored at 37oC and 100% humidity for one week to allow the materials to set completely. 18
[Table/Fig-4]: Universal testing machine [Table/Fig-5]: Mounted tooth kept on universal testing machine for fracture resistance
forces necessary to fracture each root were recorded in newtons (N). The mode of failure for each of the specimens was noted by visual inspection.
Statistical Analysis Data was analysed for significance by Analysis of Variance (ANOVA) and further pair wise comparison was performed by Bonferroni test. Level of significance was taken as 0.05.
RESULTS Mean strength of Group 1 was 212.9±55.9, Group 2 was 525.25±66.4, Group 3 was 560.5±75.4 and that of Group 4 it was 500.1±77.8 respectively. Mean of Group 1 is least followed by Group 4, Group 2 & Group 3. ANOVA tests shows that there is significant difference as p=0.000